An X-ray single crystal study of alkaline cations influence on laumontite hydration ability: II. Pressure-induced hydration of Na,K-rich laumontite
Rashchenko, Sergey V.; Seryotkin, Yurii V.; Bakakin, Vladimir V.; Microporous and Mesoporous Materials 159 (2012) 126–; doi:10.1016/j.micromeso.2012.04.029

data_1548104
_publ_section_title
;
 An X-ray single crystal study of alkaline cations influence on laumontite
 hydration ability: II. Pressure-induced hydration of Na,K-rich laumontite
;
_journal_name_full               'Microporous and Mesoporous Materials'
_journal_page_first              126
_journal_paper_doi               10.1016/j.micromeso.2012.04.029
_journal_volume                  159
_journal_year                    2012
_chemical_formula_sum
'Al7.93 Ca2.73 H31.08 K1.03 Na1.44 O63.54 Si16.07'
_chemical_formula_weight         1896.11
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 110.205(13)
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   14.813(3)
_cell_length_b                   13.1377(19)
_cell_length_c                   7.5143(6)
_cell_measurement_temperature    293(2)
_cell_volume                     1372.4(4)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_diffrn_ambient_pressure         570(50)
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.439
_diffrn_measured_fraction_theta_max 0.439
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0693
_diffrn_reflns_av_sigmaI/netI    0.0657
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            6485
_diffrn_reflns_theta_full        31.14
_diffrn_reflns_theta_max         31.14
_diffrn_reflns_theta_min         3.16
_exptl_absorpt_coefficient_mu    0.993
_exptl_crystal_density_diffrn    2.294
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             957
_refine_diff_density_max         0.516
_refine_diff_density_min         -0.425
_refine_diff_density_rms         0.106
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.089
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     125
_refine_ls_number_reflns         1011
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.089
_refine_ls_R_factor_all          0.0787
_refine_ls_R_factor_gt           0.0457
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0707P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1162
_refine_ls_wR_factor_ref         0.1255
_reflns_number_gt                682
_reflns_number_total             1011
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            lg_062_lau_abs_out.cif
_cod_data_source_block           shelxl
_cod_original_formula_sum
'H31.08 Al7.93 Ca2.73 K1.03 Na1.44 O63.54 Si16.07'
_cod_database_code               1548104